#------------------------------------------------------------------------------
#$Date: 2015-08-27 09:23:40 +0200 (jue 27 de ago de 2015) $
#$Revision: 153720 $
#$URL: svn://www.crystallography.net/cod/cif/7/22/19/7221903.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7221903
loop_
_publ_author_name
'Du, Hai-Juan'
'Wang, Chao-Hai'
'Li, Yao'
'Niu, Yunyin'
'Hou, Hongwei'
_publ_section_title
;
 Four hybrid compounds based on new type of molybdates and a flexible
 tripodal ligand: synthesis, structures, photochemical and electrochemical
 properties
;
_journal_name_full               'RSC Adv.'
_journal_paper_doi               10.1039/C5RA13007G
_journal_year                    2015
_chemical_formula_moiety         'C42 H52 Mo12 N12 O38, 4(O)'
_chemical_formula_sum            'C42 H60 Mo12 N12 O42'
_chemical_formula_weight         2556.30
_chemical_name_systematic
;
 ? 
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           61
_space_group_name_Hall           '-P 2ac 2ab'
_space_group_name_H-M_alt        'P b c a'
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2014-06-30
_audit_creation_method
;
Olex2 1.2
(compiled 2014.06.26 svn.r2951 for OlexSys, GUI svn.r4855)
;
_audit_update_record
;
2015-04-01 deposited with the CCDC.
2015-08-26 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   18.9997(3)
_cell_length_b                   14.97489(18)
_cell_length_c                   25.4844(5)
_cell_measurement_reflns_used    8616
_cell_measurement_temperature    291(2)
_cell_measurement_theta_max      28.7430
_cell_measurement_theta_min      3.3300
_cell_volume                     7250.8(2)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_diffrn_ambient_temperature      291.15
_diffrn_detector_area_resol_mean 16.2312
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_details
;
  1 omega   43.00   68.65   0.4500   11.0000
omega____ theta____ kappa____ phi______ frames
    -       19.7104   77.0000   60.0000 57

  2 omega   45.00   88.20   0.4500   11.0000
omega____ theta____ kappa____ phi______ frames
    -       19.7104   77.0000 -120.0000 96

  3 omega   51.00   76.65   0.4500   11.0000
omega____ theta____ kappa____ phi______ frames
    -       19.7104   77.0000 -180.0000 57

  4 omega    1.00   49.15   0.4500   11.0000
omega____ theta____ kappa____ phi______ frames
    -       19.7104   77.0000   90.0000 107

  5 omega  -10.00   28.25   0.4500   11.0000
omega____ theta____ kappa____ phi______ frames
    -       19.7104   77.0000   60.0000 85
;
_diffrn_measurement_device_type  'Xcalibur, Eos, Gemini'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      0.0367647000
_diffrn_orient_matrix_UB_12      0.0017664000
_diffrn_orient_matrix_UB_13      0.0047876000
_diffrn_orient_matrix_UB_21      0.0059956000
_diffrn_orient_matrix_UB_22      0.0096265000
_diffrn_orient_matrix_UB_23      -0.0268815000
_diffrn_orient_matrix_UB_31      -0.0026535000
_diffrn_orient_matrix_UB_32      0.0463212000
_diffrn_orient_matrix_UB_33      0.0054152000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0353
_diffrn_reflns_av_unetI/netI     0.0405
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_number            23355
_diffrn_reflns_theta_full        26.00
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         2.96
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    2.103
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.95046
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_density_diffrn    2.342
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             4944
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.15
_refine_diff_density_max         0.905
_refine_diff_density_min         -0.653
_refine_diff_density_rms         0.123
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.077
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     503
_refine_ls_number_reflns         7406
_refine_ls_number_restraints     29
_refine_ls_restrained_S_all      1.081
_refine_ls_R_factor_all          0.0659
_refine_ls_R_factor_gt           0.0468
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0327P)²+36.1011P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0971
_refine_ls_wR_factor_ref         0.1056
_reflns_number_gt                5838
_reflns_number_total             7406
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5ra13007g2.cif
_cod_data_source_block           exp_8320
_cod_database_code               7221903
_chemical_oxdiff_formula         C20H20N4O4Mo1
_reflns_odcompleteness_completeness 99.73
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups, All N(H) groups
 At 1.5 times of:
  All C(H,H,H) groups
2. Restrained distances
 C20-C19
 1.4 with sigma of 0.02
 N5-C19
 1.4 with sigma of 0.02
 N6-C20
 1.4 with sigma of 0.02
 C21-N6
 1.4 with sigma of 0.02
 C21-N5
 1.4 with sigma of 0.02
3. Uiso/Uaniso restraints and constraints
Uanis(C21) \\sim Ueq, Uanis(N6) \\sim Ueq, Uanis(C20) \\sim Ueq, Uanis(C19)
\\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O20) = Uanis(O20A)
4. Others
 Sof(O20A)=1-FVAR(1)
 Sof(O20)=FVAR(1)
 Fixed Sof: O21(0.5) O22(0.5)
5.a Secondary CH2 refined with riding coordinates:
 C7(H7A,H7B), C9(H9A,H9B), C11(H11A,H11B)
5.b Aromatic/amide H refined with riding coordinates:
 N4(H4), N6(H6), C13(H13), C14(H14), C15(H15), C16(H16), C17(H17), C18(H18),
 C19(H19), C20(H20), C21(H21)
5.c Idealised Me refined as rotating group:
 C8(H8A,H8B,H8C), C10(H10A,H10B,H10C), C12(H12A,H12B,H12C)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z'
2 '-x+1/2, -y, z+1/2'
3 'x+1/2, -y+1/2, -z'
4 '-x, y+1/2, -z+1/2'
5 '-x, -y, -z'
6 'x-1/2, y, -z-1/2'
7 '-x-1/2, y-1/2, z'
8 'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
Mo1 Mo 0.67098(3) -0.01110(4) 0.67342(3) 0.04546(17) Uani 1 d . . . .
Mo2 Mo 0.63645(3) -0.20835(4) 0.62560(3) 0.04682(17) Uani 1 d . . . .
Mo3 Mo 0.50926(3) -0.03524(3) 0.62404(2) 0.03201(14) Uani 1 d . . . .
Mo4 Mo 0.58729(3) 0.12999(3) 0.55864(2) 0.03483(14) Uani 1 d . . . .
Mo5 Mo 0.43132(3) 0.08005(3) 0.50414(2) 0.03007(13) Uani 1 d . . . .
Mo6 Mo 0.51101(3) 0.24112(3) 0.43911(3) 0.04194(16) Uani 1 d . . . .
O1 O 0.7327(3) 0.0683(4) 0.6617(2) 0.0626(15) Uani 1 d . . . .
O2 O 0.6943(3) -0.0574(4) 0.7321(2) 0.0639(15) Uani 1 d . . . .
O3 O 0.6952(2) -0.1030(3) 0.6261(2) 0.0471(12) Uani 1 d . . . .
O4 O 0.6596(3) -0.2560(4) 0.6834(2) 0.0684(16) Uani 1 d . . . .
O5 O 0.6782(3) -0.2688(3) 0.5789(2) 0.0621(15) Uani 1 d . . . .
O6 O 0.5745(2) -0.1319(3) 0.56255(18) 0.0357(10) Uani 1 d . . . .
O7 O 0.5715(2) -0.0919(3) 0.66786(18) 0.0399(11) Uani 1 d . . . .
O8 O 0.6020(2) 0.0429(3) 0.61195(18) 0.0364(10) Uani 1 d . . . .
O9 O 0.4489(2) -0.1200(3) 0.60925(18) 0.0384(10) Uani 1 d . . . .
O10 O 0.4629(2) 0.0354(3) 0.66179(19) 0.0424(11) Uani 1 d . . . .
O11 O 0.5492(3) 0.2115(3) 0.59505(19) 0.0485(12) Uani 1 d . . . .
O12 O 0.6671(3) 0.1721(3) 0.5433(2) 0.0546(13) Uani 1 d . . . .
O13 O 0.5301(2) 0.1510(3) 0.49525(18) 0.0357(10) Uani 1 d . . . .
O14 O 0.5000(2) 0.0250(2) 0.55272(16) 0.0300(9) Uani 1 d . . . .
O15 O 0.3760(2) -0.0112(3) 0.49732(18) 0.0381(10) Uani 1 d . . . .
O16 O 0.3862(3) 0.1492(3) 0.5436(2) 0.0489(13) Uani 1 d . . . .
O17 O 0.5909(3) 0.2873(3) 0.4271(2) 0.0628(15) Uani 1 d . . . .
O18 O 0.4697(3) 0.3144(3) 0.4797(2) 0.0593(15) Uani 1 d . . . .
O19 O 0.4583(3) 0.2612(3) 0.3780(2) 0.0484(12) Uani 1 d . . . .
N1 N 0.6036(3) 0.0781(4) 0.7193(2) 0.0426(14) Uani 1 d . . . .
N2 N 0.5474(3) 0.1955(4) 0.7488(2) 0.0480(15) Uani 1 d . . . .
N3 N 0.6422(3) 0.4783(4) 0.5807(3) 0.0490(15) Uani 1 d . . . .
N4 N 0.6910(4) 0.3881(6) 0.5268(4) 0.089(3) Uani 1 d . . . .
H4 H 0.7012 0.3406 0.5095 0.107 Uiso 1 calc . . R .
N5 N 0.3084(4) 0.3911(8) 0.6104(4) 0.104(3) Uani 1 d . . D .
N6 N 0.2060(9) 0.4212(13) 0.6132(7) 0.193(7) Uani 1 d . . D U
H6 H 0.1612 0.4133 0.6120 0.231 Uiso 1 calc . . R .
C1 C 0.5099(4) 0.3367(5) 0.7045(3) 0.0500(19) Uani 1 d . . . .
C2 C 0.5592(4) 0.4008(5) 0.6872(3) 0.0517(19) Uani 1 d . . . .
C3 C 0.5446(4) 0.4497(4) 0.6421(3) 0.0480(18) Uani 1 d . . . .
C4 C 0.4828(4) 0.4341(4) 0.6137(3) 0.0490(19) Uani 1 d . . . .
C5 C 0.4362(4) 0.3678(4) 0.6301(3) 0.0486(18) Uani 1 d . . . .
C6 C 0.4493(4) 0.3188(4) 0.6759(3) 0.051(2) Uani 1 d . . . .
C7 C 0.5235(5) 0.2879(5) 0.7557(3) 0.069(3) Uani 1 d . . . .
H7A H 0.5589 0.3204 0.7754 0.082 Uiso 1 calc . . R .
H7B H 0.4806 0.2878 0.7763 0.082 Uiso 1 calc . . R .
C8 C 0.6267(5) 0.4160(8) 0.7163(5) 0.100(4) Uani 1 d . . . .
H8A H 0.6229 0.4692 0.7371 0.150 Uiso 1 calc . . GR .
H8B H 0.6645 0.4227 0.6916 0.150 Uiso 1 calc . . GR .
H8C H 0.6361 0.3659 0.7387 0.150 Uiso 1 calc . . GR .
C9 C 0.5966(5) 0.5171(5) 0.6219(3) 0.062(2) Uani 1 d . . . .
H9A H 0.5714 0.5680 0.6076 0.075 Uiso 1 calc . . R .
H9B H 0.6256 0.5381 0.6507 0.075 Uiso 1 calc . . R .
C10 C 0.4659(6) 0.4874(6) 0.5652(4) 0.077(3) Uani 1 d . . . .
H10A H 0.4979 0.5369 0.5625 0.115 Uiso 1 calc . . GR .
H10B H 0.4185 0.5093 0.5674 0.115 Uiso 1 calc . . GR .
H10C H 0.4706 0.4500 0.5348 0.115 Uiso 1 calc . . GR .
C11 C 0.3726(5) 0.3452(7) 0.5963(4) 0.086(3) Uani 1 d . . . .
H11A H 0.3838 0.3592 0.5601 0.103 Uiso 1 calc . . R .
H11B H 0.3643 0.2814 0.5984 0.103 Uiso 1 calc . . R .
C12 C 0.4000(5) 0.2466(6) 0.6931(4) 0.083(3) Uani 1 d . . . .
H12A H 0.4135 0.1912 0.6771 0.124 Uiso 1 calc . . GR .
H12B H 0.3529 0.2616 0.6825 0.124 Uiso 1 calc . . GR .
H12C H 0.4018 0.2408 0.7305 0.124 Uiso 1 calc . . GR .
C13 C 0.5339(5) 0.1276(5) 0.7828(3) 0.064(2) Uani 1 d . . . .
H13 H 0.5065 0.1303 0.8130 0.077 Uiso 1 calc . . R .
C14 C 0.5681(4) 0.0557(5) 0.7640(3) 0.060(2) Uani 1 d . . . .
H14 H 0.5676 -0.0008 0.7792 0.072 Uiso 1 calc . . R .
C15 C 0.5882(4) 0.1632(5) 0.7118(3) 0.0464(17) Uani 1 d . . . .
H15 H 0.6044 0.1964 0.6834 0.056 Uiso 1 calc . . R .
C16 C 0.6919(4) 0.5232(5) 0.5543(3) 0.057(2) Uani 1 d . . . .
H16 H 0.7027 0.5833 0.5588 0.068 Uiso 1 calc . . R .
C17 C 0.7227(4) 0.4694(6) 0.5213(4) 0.062(2) Uani 1 d . . . .
H17 H 0.7593 0.4836 0.4985 0.074 Uiso 1 calc . . R .
C18 C 0.6419(5) 0.3952(6) 0.5632(4) 0.077(3) Uani 1 d . . . .
H18 H 0.6123 0.3497 0.5745 0.092 Uiso 1 calc . . R .
C19 C 0.3010(11) 0.4666(14) 0.6384(8) 0.201(9) Uani 1 d . . D U
H19 H 0.3382 0.4967 0.6543 0.241 Uiso 1 calc . . R .
C20 C 0.2300(11) 0.4950(15) 0.6410(8) 0.199(8) Uani 1 d . . D U
H20 H 0.2078 0.5443 0.6557 0.239 Uiso 1 calc . . R .
C21 C 0.2455(10) 0.3618(14) 0.5882(8) 0.190(8) Uani 1 d . . D U
H21 H 0.2350 0.3167 0.5644 0.229 Uiso 1 calc . . R .
O20A O 0.2693(12) 0.742(2) 0.7480(11) 0.154(6) Uani 0.394(11) d A 2 . .
O21 O 0.2898(10) 0.6983(18) 0.6446(10) 0.199(12) Uani 0.50 d . . . .
O20 O 0.2329(8) 0.6314(12) 0.7318(7) 0.154(6) Uani 0.606(11) d A 1 . .
O22 O 0.2596(9) 0.2392(16) 0.5283(9) 0.172(10) Uani 0.50 d . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Mo1 O2 105.0(3) . .
O1 Mo1 O3 103.3(2) . .
O1 Mo1 O7 161.3(2) . .
O1 Mo1 O8 91.7(2) . .
O1 Mo1 N1 94.0(2) . .
O2 Mo1 O3 101.6(2) . .
O2 Mo1 O7 93.1(2) . .
O2 Mo1 O8 158.3(2) . .
O2 Mo1 N1 86.1(2) . .
O3 Mo1 O7 76.85(18) . .
O3 Mo1 O8 87.60(19) . .
O3 Mo1 N1 158.4(2) . .
O8 Mo1 O7 69.61(15) . .
N1 Mo1 O7 82.58(18) . .
N1 Mo1 O8 78.90(19) . .
O3 Mo2 O6 83.87(18) . .
O3 Mo2 O7 72.54(17) . .
O3 Mo2 O19 148.92(18) . 5_656
O4 Mo2 O3 100.9(3) . .
O4 Mo2 O6 161.9(2) . .
O4 Mo2 O7 92.8(2) . .
O4 Mo2 O19 96.2(3) . 5_656
O5 Mo2 O3 99.8(2) . .
O5 Mo2 O4 105.3(3) . .
O5 Mo2 O6 90.8(2) . .
O5 Mo2 O7 161.4(2) . .
O5 Mo2 O19 100.5(2) . 5_656
O6 Mo2 O7 71.79(15) . .
O19 Mo2 O6 72.51(17) 5_656 .
O19 Mo2 O7 80.92(17) 5_656 .
O7 Mo3 O6 77.95(17) . .
O7 Mo3 O8 79.03(18) . .
O7 Mo3 O14 143.49(18) . .
O8 Mo3 O6 79.37(15) . .
O9 Mo3 O6 76.54(17) . .
O9 Mo3 O7 102.6(2) . .
O9 Mo3 O8 154.88(19) . .
O9 Mo3 O14 94.16(18) . .
O10 Mo3 O6 175.48(19) . .
O10 Mo3 O7 106.3(2) . .
O10 Mo3 O8 99.78(19) . .
O10 Mo3 O9 103.7(2) . .
O10 Mo3 O14 100.76(19) . .
O14 Mo3 O6 74.74(14) . .
O14 Mo3 O8 72.53(16) . .
O8 Mo4 O13 140.76(17) . .
O8 Mo4 O14 71.51(16) . .
O8 Mo4 O15 82.71(17) . 5_656
O11 Mo4 O8 99.5(2) . .
O11 Mo4 O13 95.6(2) . .
O11 Mo4 O14 102.8(2) . .
O11 Mo4 O15 171.6(2) . 5_656
O12 Mo4 O8 106.8(2) . .
O12 Mo4 O11 104.0(3) . .
O12 Mo4 O13 104.2(2) . .
O12 Mo4 O14 153.1(2) . .
O12 Mo4 O15 82.9(2) . 5_656
O13 Mo4 O14 69.90(15) . .
O13 Mo4 O15 77.91(16) . 5_656
O14 Mo4 O15 70.16(14) . 5_656
O6 Mo5 O13 75.72(17) 5_656 .
O6 Mo5 O14 141.28(17) 5_656 .
O6 Mo5 O14 76.49(15) 5_656 5_656
O13 Mo5 O14 78.27(14) . 5_656
O14 Mo5 O13 72.47(15) . .
O14 Mo5 O14 75.93(17) . 5_656
O15 Mo5 O6 101.5(2) . 5_656
O15 Mo5 O13 154.30(18) . .
O15 Mo5 O14 76.28(16) . 5_656
O15 Mo5 O14 97.72(18) . .
O16 Mo5 O6 104.9(2) . 5_656
O16 Mo5 O13 101.6(2) . .
O16 Mo5 O14 102.6(2) . .
O16 Mo5 O14 178.5(2) . 5_656
O16 Mo5 O15 103.7(2) . .
O6 Mo6 O9 70.56(15) 5_656 5_656
O13 Mo6 O6 70.26(16) . 5_656
O13 Mo6 O9 78.07(16) . 5_656
O17 Mo6 O6 156.4(2) . 5_656
O17 Mo6 O9 85.9(2) . 5_656
O17 Mo6 O13 104.0(2) . .
O17 Mo6 O18 105.1(3) . .
O17 Mo6 O19 105.2(3) . .
O18 Mo6 O6 98.2(2) . 5_656
O18 Mo6 O9 168.2(2) . 5_656
O18 Mo6 O13 94.8(2) . .
O18 Mo6 O19 98.9(2) . .
O19 Mo6 O6 73.87(18) . 5_656
O19 Mo6 O9 81.90(18) . 5_656
O19 Mo6 O13 143.02(19) . .
Mo1 O3 Mo2 117.3(2) . .
Mo2 O6 Mo3 96.06(16) . .
Mo2 O6 Mo6 91.17(14) . 5_656
Mo5 O6 Mo2 150.7(2) 5_656 .
Mo5 O6 Mo3 107.65(17) 5_656 .
Mo5 O6 Mo6 103.63(19) 5_656 5_656
Mo6 O6 Mo3 94.21(15) 5_656 .
Mo1 O7 Mo2 89.27(15) . .
Mo3 O7 Mo1 109.4(2) . .
Mo3 O7 Mo2 113.3(2) . .
Mo3 O8 Mo1 100.80(17) . .
Mo4 O8 Mo1 148.0(2) . .
Mo4 O8 Mo3 110.9(2) . .
Mo3 O9 Mo6 117.8(2) . 5_656
Mo4 O13 Mo5 108.26(19) . .
Mo4 O13 Mo6 142.5(2) . .
Mo6 O13 Mo5 104.41(19) . .
Mo3 O14 Mo4 100.53(17) . .
Mo3 O14 Mo5 101.12(15) . 5_656
Mo4 O14 Mo5 95.27(14) . 5_656
Mo5 O14 Mo3 143.1(2) . .
Mo5 O14 Mo4 103.47(16) . .
Mo5 O14 Mo5 104.07(17) . 5_656
Mo5 O15 Mo4 118.1(2) . 5_656
Mo6 O19 Mo2 117.5(2) . 5_656
C14 N1 Mo1 125.8(5) . .
C15 N1 Mo1 129.8(5) . .
C15 N1 C14 104.4(6) . .
C13 N2 C7 124.9(7) . .
C15 N2 C7 128.0(6) . .
C15 N2 C13 107.1(6) . .
C16 N3 C9 124.9(6) . .
C18 N3 C9 127.3(7) . .
C18 N3 C16 107.8(7) . .
C17 N4 H4 125.9 . .
C18 N4 H4 125.9 . .
C18 N4 C17 108.2(8) . .
C19 N5 C11 128.3(12) . .
C19 N5 C21 113.0(15) . .
C21 N5 C11 118.3(14) . .
C20 N6 H6 116.8 . .
C21 N6 H6 116.8 . .
C21 N6 C20 126.4(18) . .
C2 C1 C7 118.8(8) . .
C6 C1 C2 121.2(7) . .
C6 C1 C7 120.0(7) . .
C1 C2 C8 121.2(8) . .
C3 C2 C1 118.9(7) . .
C3 C2 C8 119.9(8) . .
C2 C3 C4 120.5(7) . .
C2 C3 C9 120.4(7) . .
C4 C3 C9 119.1(7) . .
C3 C4 C10 121.0(7) . .
C5 C4 C3 119.8(7) . .
C5 C4 C10 119.3(8) . .
C4 C5 C6 120.7(7) . .
C4 C5 C11 119.5(8) . .
C6 C5 C11 119.8(7) . .
C1 C6 C5 118.9(7) . .
C1 C6 C12 120.4(8) . .
C5 C6 C12 120.7(8) . .
N2 C7 C1 113.8(7) . .
N2 C7 H7A 108.8 . .
N2 C7 H7B 108.8 . .
C1 C7 H7A 108.8 . .
C1 C7 H7B 108.8 . .
H7A C7 H7B 107.7 . .
C2 C8 H8A 109.5 . .
C2 C8 H8B 109.5 . .
C2 C8 H8C 109.5 . .
H8A C8 H8B 109.5 . .
H8A C8 H8C 109.5 . .
H8B C8 H8C 109.5 . .
N3 C9 C3 111.4(6) . .
N3 C9 H9A 109.4 . .
N3 C9 H9B 109.4 . .
C3 C9 H9A 109.4 . .
C3 C9 H9B 109.4 . .
H9A C9 H9B 108.0 . .
C4 C10 H10A 109.5 . .
C4 C10 H10B 109.5 . .
C4 C10 H10C 109.5 . .
H10A C10 H10B 109.5 . .
H10A C10 H10C 109.5 . .
H10B C10 H10C 109.5 . .
N5 C11 C5 115.1(9) . .
N5 C11 H11A 108.5 . .
N5 C11 H11B 108.5 . .
C5 C11 H11A 108.5 . .
C5 C11 H11B 108.5 . .
H11A C11 H11B 107.5 . .
C6 C12 H12A 109.5 . .
C6 C12 H12B 109.5 . .
C6 C12 H12C 109.5 . .
H12A C12 H12B 109.5 . .
H12A C12 H12C 109.5 . .
H12B C12 H12C 109.5 . .
N2 C13 H13 126.8 . .
C14 C13 N2 106.3(7) . .
C14 C13 H13 126.8 . .
N1 C14 H14 125.1 . .
C13 C14 N1 109.8(7) . .
C13 C14 H14 125.1 . .
N1 C15 H15 123.8 . .
N2 C15 N1 112.4(7) . .
N2 C15 H15 123.8 . .
N3 C16 H16 125.3 . .
C17 C16 N3 109.3(7) . .
C17 C16 H16 125.3 . .
N4 C17 H17 126.7 . .
C16 C17 N4 106.7(7) . .
C16 C17 H17 126.7 . .
N3 C18 H18 126.0 . .
N4 C18 N3 108.0(8) . .
N4 C18 H18 126.0 . .
N5 C19 H19 124.0 . .
N5 C19 C20 112.1(18) . .
C20 C19 H19 124.0 . .
N6 C20 C19 92.9(17) . .
N6 C20 H20 133.6 . .
C19 C20 H20 133.6 . .
N5 C21 H21 132.7 . .
N6 C21 N5 94.5(15) . .
N6 C21 H21 132.7 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O1 1.696(5) .
Mo1 O2 1.706(5) .
Mo1 O3 1.887(5) .
Mo1 O7 2.248(4) .
Mo1 O8 2.197(4) .
Mo1 N1 2.189(6) .
Mo2 O3 1.933(5) .
Mo2 O4 1.694(5) .
Mo2 O5 1.693(5) .
Mo2 O6 2.297(4) .
Mo2 O7 2.392(4) .
Mo2 O19 1.969(5) 5_656
Mo3 O6 2.468(4) .
Mo3 O7 1.835(4) .
Mo3 O8 2.137(4) .
Mo3 O9 1.751(4) .
Mo3 O10 1.680(4) .
Mo3 O14 2.037(4) .
Mo4 O8 1.903(4) .
Mo4 O11 1.696(5) .
Mo4 O12 1.688(5) .
Mo4 O13 1.972(4) .
Mo4 O14 2.290(4) .
Mo4 O15 2.384(4) 5_656
Mo5 O6 1.872(4) 5_656
Mo5 O13 2.168(4) .
Mo5 O14 1.979(4) .
Mo5 O14 2.506(4) 5_656
Mo5 O15 1.733(4) .
Mo5 O16 1.679(4) .
Mo6 O6 2.306(4) 5_656
Mo6 O9 2.321(4) 5_656
Mo6 O13 2.000(4) .
Mo6 O17 1.696(5) .
Mo6 O18 1.700(5) .
Mo6 O19 1.876(5) .
O6 Mo5 1.872(4) 5_656
O6 Mo6 2.306(4) 5_656
O9 Mo6 2.321(4) 5_656
O14 Mo5 2.506(4) 5_656
O15 Mo4 2.384(4) 5_656
O19 Mo2 1.969(5) 5_656
N1 C14 1.367(9) .
N1 C15 1.320(9) .
N2 C7 1.467(9) .
N2 C13 1.360(9) .
N2 C15 1.315(9) .
N3 C9 1.480(9) .
N3 C16 1.340(9) .
N3 C18 1.322(9) .
N4 H4 0.8600 .
N4 C17 1.365(11) .
N4 C18 1.320(11) .
N5 C11 1.445(14) .
N5 C19 1.345(15) .
N5 C21 1.393(15) .
N6 H6 0.8600 .
N6 C20 1.389(16) .
N6 C21 1.327(15) .
C1 C2 1.412(10) .
C1 C6 1.388(11) .
C1 C7 1.518(11) .
C2 C3 1.391(11) .
C2 C8 1.499(12) .
C3 C4 1.399(11) .
C3 C9 1.504(10) .
C4 C5 1.395(10) .
C4 C10 1.506(11) .
C5 C6 1.401(11) .
C5 C11 1.522(11) .
C6 C12 1.495(10) .
C7 H7A 0.9700 .
C7 H7B 0.9700 .
C8 H8A 0.9600 .
C8 H8B 0.9600 .
C8 H8C 0.9600 .
C9 H9A 0.9700 .
C9 H9B 0.9700 .
C10 H10A 0.9600 .
C10 H10B 0.9600 .
C10 H10C 0.9600 .
C11 H11A 0.9700 .
C11 H11B 0.9700 .
C12 H12A 0.9600 .
C12 H12B 0.9600 .
C12 H12C 0.9600 .
C13 H13 0.9300 .
C13 C14 1.345(10) .
C14 H14 0.9300 .
C15 H15 0.9300 .
C16 H16 0.9300 .
C16 C17 1.302(11) .
C17 H17 0.9300 .
C18 H18 0.9300 .
C19 H19 0.9300 .
C19 C20 1.417(16) .
C20 H20 0.9300 .
C21 H21 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
Mo1 N1 C14 C13 177.9(6) . .
Mo1 N1 C15 N2 -177.9(5) . .
O1 Mo1 O3 Mo2 -179.2(3) . .
O1 Mo1 O7 Mo2 105.9(7) . .
O1 Mo1 O7 Mo3 -8.6(8) . .
O1 Mo1 O8 Mo3 -172.5(2) . .
O1 Mo1 O8 Mo4 0.8(5) . .
O1 Mo1 N1 C14 -140.0(6) . .
O1 Mo1 N1 C15 39.3(7) . .
O2 Mo1 O3 Mo2 72.1(3) . .
O2 Mo1 O7 Mo2 -88.0(2) . .
O2 Mo1 O7 Mo3 157.5(3) . .
O2 Mo1 O8 Mo3 -31.7(7) . .
O2 Mo1 O8 Mo4 141.6(6) . .
O2 Mo1 N1 C14 -35.2(6) . .
O2 Mo1 N1 C15 144.1(7) . .
O3 Mo1 O7 Mo2 13.17(17) . .
O3 Mo1 O7 Mo3 -101.3(2) . .
O3 Mo1 O8 Mo3 84.3(2) . .
O3 Mo1 O8 Mo4 -102.5(5) . .
O3 Mo1 N1 C14 76.7(9) . .
O3 Mo1 N1 C15 -104.0(8) . .
O3 Mo2 O6 Mo3 -79.44(17) . .
O3 Mo2 O6 Mo5 65.0(5) . 5_656
O3 Mo2 O6 Mo6 -173.80(18) . 5_656
O3 Mo2 O7 Mo1 -13.12(18) . .
O3 Mo2 O7 Mo3 97.7(3) . .
O4 Mo2 O3 Mo1 -71.8(3) . .
O4 Mo2 O6 Mo3 26.9(8) . .
O4 Mo2 O6 Mo5 171.4(7) . 5_656
O4 Mo2 O6 Mo6 -67.4(8) . 5_656
O4 Mo2 O7 Mo1 87.4(2) . .
O4 Mo2 O7 Mo3 -161.8(3) . .
O5 Mo2 O3 Mo1 -179.7(3) . .
O5 Mo2 O6 Mo3 -179.2(2) . .
O5 Mo2 O6 Mo5 -34.8(5) . 5_656
O5 Mo2 O6 Mo6 86.5(2) . 5_656
O5 Mo2 O7 Mo1 -81.0(7) . .
O5 Mo2 O7 Mo3 29.9(8) . .
O6 Mo2 O3 Mo1 90.5(3) . .
O6 Mo2 O7 Mo1 -102.30(16) . .
O6 Mo2 O7 Mo3 8.52(19) . .
O6 Mo3 O7 Mo1 90.1(2) . .
O6 Mo3 O7 Mo2 -7.70(17) . .
O6 Mo3 O8 Mo1 -88.29(17) . .
O6 Mo3 O8 Mo4 95.5(2) . .
O6 Mo3 O9 Mo6 8.1(2) . 5_656
O6 Mo3 O14 Mo4 -97.79(16) . .
O6 Mo3 O14 Mo5 -0.22(13) . 5_656
O6 Mo3 O14 Mo5 132.2(4) . .
O6 Mo5 O13 Mo4 -178.1(2) 5_656 .
O6 Mo5 O13 Mo6 20.54(18) 5_656 .
O6 Mo5 O14 Mo3 -177.5(3) 5_656 .
O6 Mo5 O14 Mo4 53.3(3) 5_656 .
O6 Mo5 O14 Mo5 -45.8(3) 5_656 5_656
O6 Mo5 O15 Mo4 69.0(2) 5_656 5_656
O6 Mo6 O13 Mo4 -167.1(4) 5_656 .
O6 Mo6 O13 Mo5 -17.05(15) 5_656 .
O6 Mo6 O19 Mo2 19.7(2) 5_656 5_656
O7 Mo1 O3 Mo2 -18.5(2) . .
O7 Mo1 O8 Mo3 7.40(16) . .
O7 Mo1 O8 Mo4 -179.3(5) . .
O7 Mo1 N1 C14 58.5(6) . .
O7 Mo1 N1 C15 -122.2(6) . .
O7 Mo2 O3 Mo1 17.7(2) . .
O7 Mo2 O6 Mo3 -5.84(13) . .
O7 Mo2 O6 Mo5 138.6(5) . 5_656
O7 Mo2 O6 Mo6 -100.20(16) . 5_656
O7 Mo3 O6 Mo2 7.40(17) . .
O7 Mo3 O6 Mo5 -155.2(2) . 5_656
O7 Mo3 O6 Mo6 99.03(18) . 5_656
O7 Mo3 O8 Mo1 -8.66(19) . .
O7 Mo3 O8 Mo4 175.1(2) . .
O7 Mo3 O9 Mo6 -66.0(3) . 5_656
O7 Mo3 O14 Mo4 -54.9(3) . .
O7 Mo3 O14 Mo5 175.1(3) . .
O7 Mo3 O14 Mo5 42.7(3) . 5_656
O8 Mo1 O3 Mo2 -88.1(3) . .
O8 Mo1 O7 Mo2 105.52(17) . .
O8 Mo1 O7 Mo3 -8.98(19) . .
O8 Mo1 N1 C14 129.1(6) . .
O8 Mo1 N1 C15 -51.6(6) . .
O8 Mo3 O6 Mo2 88.32(17) . .
O8 Mo3 O6 Mo5 -74.3(2) . 5_656
O8 Mo3 O6 Mo6 179.95(18) . 5_656
O8 Mo3 O7 Mo1 8.82(19) . .
O8 Mo3 O7 Mo2 -89.0(2) . .
O8 Mo3 O9 Mo6 25.0(6) . 5_656
O8 Mo3 O14 Mo4 -14.37(15) . .
O8 Mo3 O14 Mo5 -144.4(4) . .
O8 Mo3 O14 Mo5 83.20(16) . 5_656
O8 Mo4 O13 Mo5 28.8(4) . .
O8 Mo4 O13 Mo6 178.2(3) . .
O8 Mo4 O14 Mo3 16.27(17) . .
O8 Mo4 O14 Mo5 168.1(2) . .
O8 Mo4 O14 Mo5 -86.09(17) . 5_656
O9 Mo3 O6 Mo2 -98.87(19) . .
O9 Mo3 O6 Mo5 98.5(2) . 5_656
O9 Mo3 O6 Mo6 -7.24(17) . 5_656
O9 Mo3 O7 Mo1 163.2(2) . .
O9 Mo3 O7 Mo2 65.4(2) . .
O9 Mo3 O8 Mo1 -105.0(4) . .
O9 Mo3 O8 Mo4 78.8(5) . .
O9 Mo3 O14 Mo4 -172.62(18) . .
O9 Mo3 O14 Mo5 57.4(4) . .
O9 Mo3 O14 Mo5 -75.04(18) . 5_656
O9 Mo6 O13 Mo4 119.5(4) 5_656 .
O9 Mo6 O13 Mo5 -90.46(18) 5_656 .
O9 Mo6 O19 Mo2 91.7(2) 5_656 5_656
O10 Mo3 O6 Mo2 168(2) . .
O10 Mo3 O6 Mo5 5(2) . 5_656
O10 Mo3 O6 Mo6 -100(2) . 5_656
O10 Mo3 O7 Mo1 -88.3(2) . .
O10 Mo3 O7 Mo2 173.9(2) . .
O10 Mo3 O8 Mo1 96.2(2) . .
O10 Mo3 O8 Mo4 -80.0(3) . .
O10 Mo3 O9 Mo6 -176.5(2) . 5_656
O10 Mo3 O14 Mo4 82.6(2) . .
O10 Mo3 O14 Mo5 -47.4(4) . .
O10 Mo3 O14 Mo5 -179.82(18) . 5_656
O11 Mo4 O8 Mo1 -88.9(5) . .
O11 Mo4 O8 Mo3 84.1(3) . .
O11 Mo4 O13 Mo5 -83.7(2) . .
O11 Mo4 O13 Mo6 65.7(4) . .
O11 Mo4 O14 Mo3 -79.6(2) . .
O11 Mo4 O14 Mo5 178.02(19) . 5_656
O11 Mo4 O14 Mo5 72.2(2) . .
O12 Mo4 O8 Mo1 19.0(5) . .
O12 Mo4 O8 Mo3 -168.1(2) . .
O12 Mo4 O13 Mo5 170.4(2) . .
O12 Mo4 O13 Mo6 -40.3(4) . .
O12 Mo4 O14 Mo3 107.2(5) . .
O12 Mo4 O14 Mo5 -101.0(5) . .
O12 Mo4 O14 Mo5 4.8(5) . 5_656
O13 Mo4 O8 Mo1 159.9(3) . .
O13 Mo4 O8 Mo3 -27.2(4) . .
O13 Mo4 O14 Mo3 -171.0(2) . .
O13 Mo4 O14 Mo5 86.64(17) . 5_656
O13 Mo4 O14 Mo5 -19.21(17) . .
O13 Mo5 O14 Mo3 146.4(4) . .
O13 Mo5 O14 Mo4 17.14(15) . .
O13 Mo5 O14 Mo5 -81.91(16) . 5_656
O13 Mo5 O15 Mo4 -12.0(6) . 5_656
O13 Mo6 O19 Mo2 34.1(5) . 5_656
O14 Mo3 O6 Mo2 162.93(18) . .
O14 Mo3 O6 Mo5 0.30(17) . 5_656
O14 Mo3 O6 Mo6 -105.44(17) . 5_656
O14 Mo3 O7 Mo1 47.9(4) . .
O14 Mo3 O7 Mo2 -49.9(4) . .
O14 Mo3 O8 Mo1 -165.5(2) . .
O14 Mo3 O8 Mo4 18.32(19) . .
O14 Mo3 O9 Mo6 81.3(2) . 5_656
O14 Mo4 O8 Mo1 170.7(5) . .
O14 Mo4 O8 Mo3 -16.33(17) . .
O14 Mo4 O13 Mo5 17.91(15) . .
O14 Mo4 O13 Mo6 167.3(4) . .
O14 Mo5 O13 Mo4 -99.29(19) 5_656 .
O14 Mo5 O13 Mo4 -20.52(18) . .
O14 Mo5 O13 Mo6 99.40(19) 5_656 .
O14 Mo5 O13 Mo6 178.2(2) . .
O14 Mo5 O14 Mo3 -131.7(4) 5_656 .
O14 Mo5 O14 Mo4 99.06(19) 5_656 .
O14 Mo5 O14 Mo5 0.0 5_656 5_656
O14 Mo5 O15 Mo4 -3.86(19) 5_656 5_656
O14 Mo5 O15 Mo4 -77.3(2) . 5_656
O15 Mo4 O8 Mo1 99.3(4) 5_656 .
O15 Mo4 O8 Mo3 -87.8(2) 5_656 .
O15 Mo4 O13 Mo5 90.98(18) 5_656 .
O15 Mo4 O13 Mo6 -119.7(4) 5_656 .
O15 Mo4 O14 Mo3 105.04(18) 5_656 .
O15 Mo4 O14 Mo5 -103.2(2) 5_656 .
O15 Mo4 O14 Mo5 2.68(13) 5_656 5_656
O15 Mo5 O13 Mo4 -91.2(5) . .
O15 Mo5 O13 Mo6 107.5(4) . .
O15 Mo5 O14 Mo3 -58.0(4) . .
O15 Mo5 O14 Mo4 172.75(18) . .
O15 Mo5 O14 Mo5 73.69(19) . 5_656
O16 Mo5 O13 Mo4 79.2(2) . .
O16 Mo5 O13 Mo6 -82.1(2) . .
O16 Mo5 O14 Mo3 48.0(4) . .
O16 Mo5 O14 Mo4 -81.2(2) . .
O16 Mo5 O14 Mo5 179.70(19) . 5_656
O16 Mo5 O15 Mo4 177.7(2) . 5_656
O17 Mo6 O13 Mo4 36.9(4) . .
O17 Mo6 O13 Mo5 -173.1(2) . .
O17 Mo6 O19 Mo2 175.2(3) . 5_656
O18 Mo6 O13 Mo4 -70.0(4) . .
O18 Mo6 O13 Mo5 80.0(2) . .
O18 Mo6 O19 Mo2 -76.4(3) . 5_656
O19 Mo2 O3 Mo1 50.3(5) 5_656 .
O19 Mo2 O6 Mo3 80.11(18) 5_656 .
O19 Mo2 O6 Mo5 -135.5(5) 5_656 5_656
O19 Mo2 O6 Mo6 -14.25(17) 5_656 5_656
O19 Mo2 O7 Mo1 -176.76(19) 5_656 .
O19 Mo2 O7 Mo3 -65.9(2) 5_656 .
O19 Mo6 O13 Mo4 178.2(3) . .
O19 Mo6 O13 Mo5 -31.8(4) . .
N1 Mo1 O3 Mo2 -37.0(7) . .
N1 Mo1 O7 Mo2 -173.62(19) . .
N1 Mo1 O7 Mo3 71.9(2) . .
N1 Mo1 O8 Mo3 -78.7(2) . .
N1 Mo1 O8 Mo4 94.5(5) . .
N2 C13 C14 N1 1.0(11) . .
N3 C16 C17 N4 0.6(11) . .
N5 C19 C20 N6 3(2) . .
C1 C2 C3 C4 -1.3(11) . .
C1 C2 C3 C9 -178.6(7) . .
C2 C1 C6 C5 -2.2(10) . .
C2 C1 C6 C12 176.2(7) . .
C2 C1 C7 N2 -104.9(9) . .
C2 C3 C4 C5 -1.5(11) . .
C2 C3 C4 C10 179.2(7) . .
C2 C3 C9 N3 95.6(9) . .
C3 C4 C5 C6 2.5(10) . .
C3 C4 C5 C11 -174.2(7) . .
C4 C3 C9 N3 -81.7(9) . .
C4 C5 C6 C1 -0.7(10) . .
C4 C5 C6 C12 -179.1(7) . .
C4 C5 C11 N5 -94.5(11) . .
C6 C1 C2 C3 3.2(11) . .
C6 C1 C2 C8 -176.1(8) . .
C6 C1 C7 N2 76.1(10) . .
C6 C5 C11 N5 88.7(11) . .
C7 N2 C13 C14 -176.5(8) . .
C7 N2 C15 N1 175.4(8) . .
C7 C1 C2 C3 -175.9(7) . .
C7 C1 C2 C8 4.8(11) . .
C7 C1 C6 C5 176.9(6) . .
C7 C1 C6 C12 -4.8(10) . .
C8 C2 C3 C4 178.0(8) . .
C8 C2 C3 C9 0.7(12) . .
C9 N3 C16 C17 179.4(8) . .
C9 N3 C18 N4 -179.6(8) . .
C9 C3 C4 C5 175.9(6) . .
C9 C3 C4 C10 -3.4(11) . .
C10 C4 C5 C6 -178.2(7) . .
C10 C4 C5 C11 5.1(11) . .
C11 N5 C19 C20 175.7(15) . .
C11 N5 C21 N6 178.9(12) . .
C11 C5 C6 C1 176.1(7) . .
C11 C5 C6 C12 -2.3(11) . .
C13 N2 C7 C1 -149.1(8) . .
C13 N2 C15 N1 -0.9(9) . .
C14 N1 C15 N2 1.5(9) . .
C15 N1 C14 C13 -1.5(9) . .
C15 N2 C7 C1 35.3(13) . .
C15 N2 C13 C14 -0.1(10) . .
C16 N3 C9 C3 177.7(8) . .
C16 N3 C18 N4 0.6(11) . .
C17 N4 C18 N3 -0.2(12) . .
C18 N3 C9 C3 -2.0(13) . .
C18 N3 C16 C17 -0.8(11) . .
C18 N4 C17 C16 -0.3(12) . .
C19 N5 C11 C5 20(2) . .
C19 N5 C21 N6 -8(2) . .
C20 N6 C21 N5 12(3) . .
C21 N5 C11 C5 -167.9(12) . .
C21 N5 C19 C20 3(3) . .
C21 N6 C20 C19 -10(3) . .
